**HAL Id: hal-02394300**

**https://hal.archives-ouvertes.fr/hal-02394300**

### Submitted on 4 Dec 2019

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

**Hysteresis**

### D. Mukherjee, K. Danas

**To cite this version:**

### D. Mukherjee, K. Danas. An Evolving Switching Surface Model for Ferromagnetic Hysteresis. Journal

### of Applied Physics, American Institute of Physics, 2019, 125 (3), pp.033902. �10.1063/1.5051483�.

### �hal-02394300�

D. Mukherjee1_{and K. Danas}1,a)

LMS, C.N.R.S, ´Ecole Polytechnique, Palaiseau, 91128, France (Dated: 22 November 2019)

We propose a thermodynamically consistent rate-independent three-dimensional model of magnetic hysteresis in terms of energetic and dissipation potentials making use of a relatively small number of model parameters that is capable of being implemented in a general incremental numerical setting. The dissipation process occurring during magnetization/demagnetization is described by a power-law potential, which leads to rate-independence at a certain limit of the rate-dependent exponent. The incorporation of isotropic hardening in the model enables us to describe phenomenologically at the macroscopic scale both nucleation and pinning type constitutive responses. We further model the symmetric and asymmetric minor loops by employing the idea of a bounding surface, which was originally introduced in the context of mechanical plasticity. Our model shows a very good agreement with experiments for spark plasma sintered NdFeB magnets, where nucleation is found to be the primary mechanism of coercivity. We also use our model to probe experiments for melt-spun NdFeB ribbons and powders, where both nucleation and pinning mechanisms are experimentally found to be significant. Moreover, we correlate the proposed model parameters with the underlying mechanisms for coercivity. Finally, we probe the predictive capability of the proposed model by first fitting an experimental minor loop, and then use it to successfully predict the remaining minor loops, obtained from that experiment. We also construct a FORC diagram for the floppy disc material and compare it with the corresponding experimental data.

Keywords: Thermodynamic potentials, Ferromagnetic switching, Bounding surface

I. INTRODUCTION

Recent developments in the manufacturing of rare
earth (RE) metal based polycrystalline permanent
magnets1–6 _{and recent experiments with RE magnetic}

particle filled magnetorheological elastomers (MREs)7–10
open a vast window of opportunity for designing different
microstructures to achieve specific magnetic properties
at the macroscale. Theoretical modeling of the
macro-scopic behavior of metallic magnets/MREs requires
effi-cient constitutive models, which must be
thermodynam-ically consistent at the same time. In this regard,
Hu-ber11 _{proposed such a model for ferroelectric materials}

that exhibits hysteresis, in terms of an energetic
poten-tial and a switching surface, which defines the
bound-ary of the energetic/switching response. This
switch-ing surface model has been modified later by Cocks and
Mcmeeking12_{, McMeeking and Landis}13_{, Landis}14 _{and}

Klinkel15_{and has been used extensively in finite element}

computations of dissipative electro/magneto mechanical
materials16,17_{. The switching surface idea can be directly}

related to the coercivity of a magnet, which serves to describe the effect of complex domain wall motion and interaction at the macroscale.

Specifically, coercivity constitutes one of the most im-portant dissipative mechanisms in permanent magnets. The magnetic field, that is required to demagnetize a magnet completely from a fully magnetized (saturated) state is the coercive field, which is, in turn, the mea-sure of coercivity. Experiments show two different kinds

a)_{Electronic mail:}_{konstantinos.danas@polytechnique.edu}

of coercivity mechanisms in hard magnets; (a) magnetic
domain nucleation and (b) magnetic domain pinning.
Most of the hard magnets in nature are found to
mag-netize/demagnetize through a combined effect of domain
nucleation and domain wall pinning. The type of a
mag-net is determined based on the mechanism that is
domi-nant. For example, in sintered RE magnets like NdFeB,
nucleation is found to be dominant18–22_{, whereas, in most}

of the steels like Si steel, MnMg steel, the coercivity arises
due to domain wall pinning23_{. Recent experiments by Li}

et al.24 _{have shown that both nucleation and pinning}

mechanisms play equally important roles in the magneti-zation/demagnetization of melt-spun NdFeB ribbons and powders.

Magnetic domain nucleation is a phenomena where
re-verse magnetic domains nucleate near the crystal defects.
This mechanism ensures high susceptibility at the
begin-ning of magnetization and consequently, magnetic
satu-ration is achieved at a lower magnetic field18–20.
Exper-iments by Huang et al.6 _{confirm the nucleation }

mech-anism in sintered NdFeB magnets by showing that vir-gin state sintered NdFeB magnets do exhibit high sus-ceptibility at the beginning. Kronm¨uller, Durst, and Sagawa18 show that the micromagnetic domain proper-ties and temperature dependence of the coercive field in sintered NdFeB magnets are direct consequences of do-main nucleation.

In turn, most of the traditional ferromagnetic materials
like steel and Fe-Ni-Co alloys exhibit a coercivity
mech-anism known as domain wall pinning25_{. In this case, the}

magnetic domains remain strongly pinned to the crys-tal grain boundaries, and as a result the initial mag-netic susceptibility during magnetization remains low. At the onset of switching, the domain walls get unpinned

from the defects and consequently, reversed domains
ro-tate quickly towards the direction of the magnetic field,
causing a rapid increase in the magnetization, termed as
magnetic switching16,17_{. Notably, for pinning-type }

mag-nets the switching starts after the local magnetic field reaches a threshold, whereas, for nucleation-type mag-nets, the switching starts even under a very small local field. This key idea of early initiation of the magnetic switching plays a pivotal role in defining the evolution of the magnetic switching surface, which is investigated in detail in this paper.

During the initial development of macroscopic
consti-tutive models of ferromagnetic hysteresis, most of the
magnets were made of steel. Thus, early experiments
with steels23 _{mostly show a pinning-type initial }

mag-netization response. Hence, classical hysteresis models
like the Preisach26 and Jiles and Atherton27 models are
based on the domain wall pinning theory. Moreover, it
is very difficult to establish thermodynamic consistency
of these models in complex non-uniaxial loading
histo-ries. In view of this, one can categorize the
thermody-namically consistent models for ferro-electric/magnetic
hysteresis under two broad distinct classes. The first
class28–31considers a double well energetic potential
asso-ciated with a ferro-electric/magnetic single crystal. Such
models allow the single crystals to switch between two
distinct states of polarization/magnetization (similar to a
phase transition). Various homogenization32–34 and
sta-tistical averaging31,35,36 techniques have been employed
to extend such single-crystal switching laws to model
polycrystalline ferro-electrics/magnets. In those
mod-els, it is very difficult to obtain intermediate
polariza-tion/magnetization in-between the two extremities of
the coersive response. Nevertheless, experiments show
that the ferro-electric/magnetic single crystals and
espe-cially polycrystals do exhibit such intermediate
polariza-tion/magnetization states37,38_{. Thus, a second class of}

more phenomenological models11,12_{have been proposed.}

The latter are based on a convex energetic potential and
a switching surface (similar to yield surface in mechanical
plasticity), that dictates the dissipative behavior of the
single crystals. Extension of such single crystal plasticity
models to polycrystalline materials is typically obtained
either through homogenization37 or by proposing
consti-tutive laws based on a convex potential and a switching
surface, directly at the macro scale13–16_{.}

Even more interestingly, complex symmetric and
asymmetric minor loops are also observed in a magnet
either due to fully reversed loading cycles with amplitude
less than the coercive field, or due to partially reversed
cycles. The minor loops are typically modeled by
intro-ducing a set of history-dependent parameters in the
clas-sical Jiles and Atherton27 _{model}39,40_{. However, those}

models are not based on energetic and dissipation po-tentials and thus their thermodynamic consistency (and positive magnetic dissipation) is extremely difficult to be addressed for all possible loadings, including cyclic ones. On the other hand, the double-well potential-based

Bergqvist31 model and its successors35,36,41,42 trace the
minor loops, but again, no clear connection between the
minor loops and the loading history is established by
these models. In turn, the existing macroscopic
switch-ing surface models13–16 _{have only been used so far to}

model the outer coersive response but have not been
ex-tended to accurately model such minor loops. Such minor
loops and incomplete magnetized responses are expected
to be extremely important in recently fabricated NdFeB
particle-filled elastomers42_{, which constitute novel }

ma-terials with great potential technological applications in sensors and actuators, as well as in haptic devices.

In view of this, following the works of Landis14 and
Klinkel15, we propose here a thermodynamically
consis-tent model by use of frame-invariant free energy functions
and dissipation potentials, thus ensuring positive work
during any loading history. In addition, we model the
mi-nor loops by evolving the switching surface as a function
of a set of history-dependent state variables. Those
vari-ables mimic (mechanical) plasticity and specifically the
notion of the bounding surface proposed by Dafalias and
Popov43 _{(see also}44,45_{). Following this idea, Chaboche,}

Van, and Cordier46_{proposed a bounding surface that lies}

in the plastic strain space (see comprehensive review47).
In this work, we extend the latter key idea in the context
of ferromagnetism by introducing internal variables such
as the accumulated remanent h-field, as well as a number
of proximity variables serving to measure and memorize
the distance of the actual h−field from the outer
bound-ing surface. The complete set of variables is employed
to model the initial magnetization, the fully magnetized
coersive loop and ultimately symmetric and asymmetric
first order minor loops in magnetic polycrystalline
ma-terials. In the case of no initial magnetization and no
minor loops, the present model fully recovers the models
of Landis14 _{and Klinkel}15_{.}

We organize this article as follows. In SectionIIwe re-call the fundamental governing Maxwell’s equations for magnetism and define the relevant variables of the prob-lem. In Section III, we develop a thermodynamically consistent constitutive model with hysteresis by defin-ing the general thermodynamic framework for dissipative systems. In SectionIII A, we propose a hardening func-tion during magnetic switching and then define an ap-propriate isotropic hardening function in Section III B. The idea of a bounding surface in the remanent h-field space is developed in Section IV A. In SectionIV B, we introduce specific modifications in the evolution law of the switching surface. A detailed account of the identi-fication of model parameters are given in Section V In SectionVI, we carry out an extensive assessment of the proposed model, by probing available hysteresis data for RE-based NdFeB magnets, Co alloys, and different kind of steels. Finally, we summarize our work and draw the conclusions in SectionVII.

II. PRELIMINARY DEFINITIONS

We consider a static and non-deformable magnetic solid occupying a volume Ω0 in the three dimensional Euclidean space. In the absence of mechanical deforma-tions, electric fields and free charges, the local magnetic field b and the local h-field h in Ω0 are governed by the following field equations

div b = 0, curl h = 0, (1) respectively. One can then define the magnetization vec-tor per unit current volume m in terms of b and h by

b = µ0(h + m). (2)

Here, µ0 is the magnetic permeability in vacuum. The curl-free property of the h-field in Ω0allows us to express h as the gradient of a scalar potential ϕ, i.e. h = −∇ϕ. Similarly, the divergence-free b may be expressed as the curl of a vector potential α, i.e., b = curlα.

The magnetic response of a solid may be modeled by
using either b or h (together with m) as the primary
vari-able. Some of the existing models use either b48–51_{, or}

m and b42,52_{as the primary variable. However, from the}

computational point of view, the choice of the curl-free
h-field as the primary variable has the advantage of
re-quiring only a scalar potential field ϕ. As a result, most
of the existing computational frameworks for magnetic
solids have been developed in the h framework16,17,53_{.}

In the present work, we also use h as the primary vari-able in our model to ensure an efficient computational framework. The dependent variable b is then obtained as a function of h by using the proposed magnetic con-stitutive law. The magnetization may then be computed from (2).

III. THE CONSTITUTIVE MODEL FOR SYMMETRIC

CYCLIC LOADING

Air and other magnetically inert media with no
mag-netization, are typically modeled by a linear constitutive
relation b = µ0h. The constitutive relation for
mag-netically soft iron with no significant hysteresis is
typi-cally given by an inverse sigmoid function like the inverse
Langevin function or the inverse hyperbolic tangent
func-tion or any combinafunc-tion of them51_{. In turn, the }

constitu-tive modeling of hard magnets that dissipate energy via hysteresis is not straightforward. To this end, we split h into an energetic part heand a dissipative part hr, called the remanent h-field, such that

h = he+ hr. (3)

The magnetic response is then described in terms of a
Helmholtz free energy ψ. Following McMeeking and
Lan-dis13 _{and Klinkel}15_{, we propose an additive }

decomposi-tion of the Helmholtz free energy into energetic and re-manent parts, such that

ρ0ψ(h, hr) = ρ0ψe(h, hr) + ρ0ψr(hr), (4)

where ρ0 is the reference density of the material. In the
above expression, ψe _{is the free energy associated with}
the energetic response, whereas ψr _{is associated to the}
remanent hr_{. Specifically, the energetic response of the}
magnet is taken to be quadratic in he _{= (h − h}r_{), such}
that

ρ0ψe= − 1 2(h − h

r_{) · µ · (h − h}r_{).} _{(5)}

In this expression, µ denotes the permeability tensor, which becomes µI for isotropic magnets (with I denoting the second order identity tensor). The magnetic field b is then obtained from the constitutive relation as

b = −ρ0
∂ψ
∂h = −ρ0
∂ψe
∂h = µ · (h − h
r_{).} _{(6)}

Furthermore, the back magnetic field bb _{(in analogy to}
back stress in mechanics) is defined as

bb = −ρ0 ∂ψr

∂hr. (7)

We note at this point that Landis14 also came up with a
similar term called the back electric field in the context
of ferroelastic ceramics. The back field is typically taken
to be an inverse sigmoid function of hr14,15_{. The }

spe-cific choice of ψr _{depends on the phenomenology of the}
magnet and is discussed later in SectionIII A.

From the second law of thermodynamics, we obtain the dissipation inequality for an isothermal, non-deforming magnetic solid as13–15

D:= −ρ0ψ − b · ˙˙ h ≥ 0, (8)

where ( ˙ ) denotes the material time derivative and D is
the dissipative power11_{. Expanding ˙}_{ψ in (}_{8}_{) yields}

D=
− ρ0
∂ψ
∂h − b
· ˙h +
− ρ0
∂ψ
∂hr
· ˙hr_{≥ 0.} _{(9)}
Substituting (6) to the above leads to

D= −ρ0 ∂ψ ∂hr· ˙h

r_{= b}r

· ˙hr≥ 0. (10)
Here, we have introduced the notion of the remanent
magnetic field, br_{, which is the work conjugate of ˙}_{h}r_{.}
The former can be written in terms of the actual
mag-netic field b minus the back magmag-netic field bb_{, i.e.,}

br= −ρ0
∂ψ
∂hr = −b − ρ0
∂ψr
∂hr = −b + b
b_{.} _{(11)}

The remanent field br _{can be expressed in terms of ˙}_{h}r
through the dissipation potentialD via

br= ∂D

∂ ˙hr. (12)

Equation (11) and (12) lead to the Generalized Standard
Material54,55 _{(GSM) relation}
ρ0
∂ψ
∂hr +
∂D
∂ ˙hr = 0. (13)

The above constitutive relations can of course be ob-tained in an inverse manner, i.e., starting by the GSM framework and work out the various equations resulting from that. Note thatD must be a convex function of ˙hr in order to satisfy the inequality (10) and thus lead to positive magnetic work. In the following, we propose a specific functional form ofD.

The energy dissipated during the magnetic domain
switching is modeled by use of a convex power-law
dis-sipation potential. This potential serves as the
macro-scopic phenomenological representation of the energy
associated with the collective irreversible domain wall
motions56,57 _{at the microscale. In particular, we }

con-sider a visco-switching response of the magnet and define a strictly convex power-law dissipation potential by58

D( ˙hr_{) =} ˙hr0bc(ξN)
m + 1
| ˙hr_{|}
˙hr
0
!m+1
. (14)
In this expression, ˙hr

0 is a reference h-field rate and m is the rate sensitivity parameter taking values between 1 (linear rate-dependent) and 0 (rate-independent switch-ing surface). The convexity of D in (14) guarantees a positive magnetic work. In order to model complex load-ing histories as well as non-trivial hardenload-ing responses, the coercive field bc is considered to be a function of N history-dependent variables, denoted compactly by using the set ξN. The elements of ξ will be defined later in the SectionsIII Band IV A. The scalar parameter, bc, serves to describe in a phenomenological manner the coercivity mechanisms found in different permanent magnets and is discussed in detail in SectionIII B.

The Legendre transform of the strictly convex D( ˙hr_{)}
with respect to ˙hr _{is defined by}

D∗_{(b}r_{) = sup}
˙
hr

h

br· ˙hr_{−}_{D( ˙h}r_{)}i_{.} _{(15)}
The maximization operation in the above definition leads
to (12), which, in turn, allows to compute ˙hr_{in terms of}
brand substitute it back to (14) to obtain

D∗_{(b}r_{) =} ˙hr0bc(ξN)
n + 1
|br_{|}
bc(ξN)
!n+1
, (16)
or
˙
hr=∂D
∗
∂br = ˙h
r
0
|br_{|}
bc(ξN)
!n
br. (17)

Here, n = 1/m such that n = 1 leads to a linear rate-dependent response. In the limit of n → ∞, which is of interest in the present work, the dissipation potential becomes convex and reads

D∗_{(b}r_{) =} 0, |br| ≤ bc(ξN)

∞, otherwise. (18)

This allows for the definition of the ferromagnetic
switch-ing surface14–16 _{which reads}

φ(br, ξN) := br· br− bc(ξN)2. (19)
This expression corresponds to a spherical switching
sur-face in the br−space with a radius equal of that
pre-scribed by the coercive field bc. The history-dependent
variable switching surface (19) is a straightforward
ex-tension of existing models in the context of ferroelectric
switching14,15_{, where b}

c is taken to be constant. The evolution of the switching surface with ξN is discussed in SectionsIII BandIV B.

Finally, we obtain the associated switching rule from (19) as

˙

hr= ˙λ ∂φ

∂br, (20)

where ˙λ is a scalar multiplier with ˙λ > 0 when φ = 0 and ˙λ = 0 when φ < 0 (seeAppendixfor details).

It is relevant to mention here that the present work fo-cuses on the modeling of rate-independent (quasi-static) hysteresis in ferromagnetic materials, i.e. the n → ∞ limit. Its extension to a rate-dependent response can be obtained by setting 1 < n ∞ in (16). Unfortunately, there exist no experimental data in the literature for rate-dependent hysteresis under slowly/moderately changing h-field to assess the more general model in those cases.

A. Energetic hardening functions

The choice of the hardening function is crucial for
ob-taining an accurate constitutive response. In this section,
we propose a specific functional form for ψr_{(h}r_{) to }
ob-tain the back magnetic field bb _{in terms of h}r_{. Similar}
phenomenological models for ferroelectric switching
con-sider the back electric displacement field db _{to be an }
in-verse sigmoid function of the local remanent electric field
er13,15–17_{. In this regard, we propose a ψ}r_{(h}r_{), which}
is a combination of a logarithmic and inverse hyperbolic
tangent functions such that

ρ0ψr(hr) =
1
2h
r_{· µ · h}r_{− κψ}
log(hr)
− (1 − κ)ψtanh(hr), 0 ≤ κ ≤ 1, (21)
with
ψlog(hr) = K1hrs
log
1 − |h
r_{|}
hr
s
+|h
r_{|}
hr
s
(22)
and
ψtanh(hr) = K1hrs
|hr_{|}
hr
s
tanh−1 |h
r_{|}
hr
s
+1
2log
hr
hr
s
·h
r
hr
s
− 1
. (23)

FIG. 1: Hard magnetic response for different κ = 0 and κ = 1.

Here, hr_{s}is the saturation hr-field and K1, κ are hysteresis
shape parameters. In the two special cases
correspond-ing to κ = 1 and κ = 0, (21) reduces to the hardening
functions of Landis14 _{and Klinkel}15_{, respectively. }

Sub-stituting (21), (22) and (23) into (11), we obtain

br= −µ · h − K1
κ h
r_{/h}r
s
1 − |hr_{|/h}r
s
+ (1 − κ) tanh−1 |h
r_{|}
hr
s
hr
|hr_{|}
.
(24)

Depending on whether κ = 1 or 0, (24) reduces to
an inverse sigmoid function of the type x/(1 − |x|) or
tanh−1(x), respectively. The last relation along with (19)
and (20) are used to compute the evolution of hr _{for a}
given variation of the applied magnetic field h (see
Ap-pendixfor details).

For illustration purposes, we show in Fig.1entire m−h
hysteresis loop as obtained by the previously discussed
definitions. We apply h = h_{b}e1 (such that hr = hrbe1)
and consider the two special cases κ = 1 and κ = 0
corresponding to (22) and (23), respectively. We find
a sharper increase of m when κ = 0, whereby κ = 1
leads to a smoother S-shaped hysteresis loop. In practice,
the choice of the interpolation parameter 0 ≤ κ ≤ 1
is made in accord with the available experimental
m-h response of tm-he magnet, as discussed in detail in tm-he
Results SectionV.

Before we proceed further, it is useful to introduce the anhysteretic approximations of the above proposed dis-sipative response. For simplicity, we assume an isotropic magnetic response with µ = µI and write51

b =
µ
h + hr
stanh
_{µ}
K1
|h| h
|h|
, κ = 0
µ
h + hr_{s}
µh/K1
1 + µ|h|/K1
, κ = 1.
(25)

FIG. 2: Soft magnetic response in the limit of bmaxc → 0 and comparison with the corresponding anhysteretic

constitutive laws.

Those purely energetic expressions lead to a typical sat-urating magnetization response in the m-h space. Using (25) along with (2), we obtain the magnetization

m =
mstanh
_{µ}
K1
|h| h
|h|, κ = 0
ms
_{µh/K}
1
1 + µ|h|/K1
, κ = 1,
(26)
where
ms= hrs/(1 − χ
(r)_{),} _{(27)}

is the saturation magnetization. The parameter χ(r) = 1 − µ0/µ denotes the relative susceptibility and µ0 = 4π × 10−7 is the permeability of air. Such an anhystr-ertic constitutive response is typically employed in the modeling of soft magnets like the carbonyl iron powder51

or cobalt ferrite59. Note that, the purely energetic ap-proximation of (25) for weakly dissipative magnets can be obtained by considering bc → 0 in (19). However, such an approximation is only a mathematical opera-tion that allows to recover equaopera-tion (25). This has no physical ground since in practice there exist no magnet, whose bc is identically zero. As shown in Fig.2, the soft (anhysteretic) magnetic response can be readily obtained from the proposed dissipative framework by use of small values of bmax

c . Those weakly hysteretic curves can be
approximated by the corresponding anhysteretic
consti-tutive laws (26) for simplicity in analysis. Figure2clearly
indicates that as bmax_{c} goes to zero, the constitutive law
reduces to that in equation (26).

B. Isotropic hardening and symmetric cyclic loading

In this section, we discuss in detail the evolution of the coercive field bc(ξN) in terms of two history-dependent internal variables (N = 2), namely, ξ2≡ {¯hr, Rhr}. The

first element of ξ2 is the accumulated remanent h-field (similar to the accumulated plastic strain in mechanical plasticity), defined as

˙¯hr_{=}p ˙hr_{· ˙h}r_{,} ¯_{h}r_{=}Z
t

˙¯hr_{dt.} _{(28)}
The second element of ξ2 is the radius of the memory
surface, which is discussed later in this section.

Initial magnetization and hardening

It is important to note at this point that in spite of exhibiting a qualitatively similar major hysteresis loop, the underlying mechanisms behind the ferroelectric and ferromagnetic switching differ significantly. The ferro-electrics undergo a phase transition upon loading beyond a critical electric field leading to switching of the polar-ization direction within a ferroelectric crystal37.

On the other hand, the ferromagnets consist of a large
number of magnetic domains with different directions of
magnetization, whereas domain nucleation and domain
wall pinning are the two key mechanisms that cause
coer-civity. Experiments and micromagnetic theories suggest
that the coercivity in RE magnets arise due to a
com-bined effect of domain wall pinning and nucleation60_{. It}

is observed through advanced imaging techniques that
reversed domains nucleate right from the beginning of
magnetization of a virgin NdFeB specimen24_{. Thus, a}

combination of nucleation and pinning causes consider-able amount of initial magnetization as compared to a solely pinning-type magnet. In order to capture this mi-croscopic phenomena at the mami-croscopic level, we con-sider that the switching surface (19) evolves from a very small radius b0

c to a constant limiting surface of radius bmax

c , which is the saturation coercive field, as shown in Fig.3a(inset). Motivated by experimental results then, the switching surface radius is a function of ¯hr (i.e., the first element of ξ2) and can take the following form

bc(¯hr) = bmaxc
tanh
¯_{h}r
¯
hr
0
81/q
. (29)
In this expression, ¯hr

0 is a reference accumulated
rema-nent field (in analogy to the yield strain in mechanical
plasticity) and q is a hardening exponent. The above
evolution law for the switching surface is qualitatively
similar to the isotropic hardening rules in mechanical
plasticity46,47_{. As a consequence of the constitutive }

rela-tion (29), the magnetic domain nucleation is now cap-tured by allowing switching right from the beginning. Obviously, the hardening exponent q plays a pivotal role

in the modeling of different coercivity mechanisms at the
macroscopic level. For a better understanding of this
parameter, we discuss a few representative cases in the
context of Fig. 3. We note first that for q → ∞, the
coercive field bc(¯hr) → bmaxc , which, indeed, models the
pinning type magnets. Thus, in the limit of q → ∞,
the proposed model reduces to the existing ferroelectric
switching models13–17_{with no isotropic hardening.}

On the other hand, a pure nucleation-type response is obtained for q = 1. In this case, as depicted in in Fig.3a,b, the switching surface starts growing from a ra-dius bc≈ 0 at a and then evolves through intermediate switching surfaces like b to finally saturate to the limit-ing surface of radius bmax

c at c . Practically, ferromagnets are modeled by choosing values in the range 1 ≤ q < ∞ as there exist no magnet that exhibits only pure domain pinning or only pure domain nucleation.

Cyclic loading and symmetric minor loops

The symmetric minor loops are obtained whenever the loading/unloading amplitude is kept below the saturation h-field hs. Note that the magnetic domains do not be-come fully aligned to the loading direction before satura-tion. Thus, if a load reversal takes place at |h| < hs, then a lower h-field is required to reverse the specimen’s mag-netization direction. The minor loops during the initial magnetization of a specimen can be obtained in the pro-posed phenomenological framework by suitably defining the accumulated remanent field ¯hr. Note further that ¯hr is a strictly increasing, history-dependent variable, which controls the evolution of the coercive filed bc. In order to capture the symmetric minor loops, we introduce a new history-dependent internal variable Rhr (i.e., the second

element of ξ2) that memorizes the prior maximum
re-manent field range. The notion of such a rere-manent field
range memory variable was first introduced by Chaboche,
Van, and Cordier46 _{in the context of cyclic mechanical}

plasticity. Following Chaboche47_{, we allow ˙¯}_{h}r _{to evolve}
following equation (29) only if the state of hrlies on the
memory surface. The latter is a spherical surface (for
isotropic magnets) of radius Rhr defined in the hr-space

by

φm:= hr· hr− R2hr. (30)

At a given instant t0, Rhr corresponds to the maximum

amplitude that hr has reached over the entire loading history up to that time instant, i.e.,

Rhr = max ||hr(t)||, ∀0 < t < t_{0}. (31)

The isotropic hardening is effective only if the local state of hr lies on the memory surface φm. This feature is incorporated in the hardening rule (29) by modifying (28) as

˙¯hr_{=} p ˙hr· ˙hr, if φm= 0
0, if φm< 0.

FIG. 3: (a)(inset) Evolving switching surface (in 2D) from a radius of b0

c to bmaxc . (a) Variation of bc with ¯hr for different hardening exponents. (b) Effect of hardening exponent q on the initial magnetization curve.

Note that bc in (29) is not an explicit function of Rhr.

However, Rhr controls the evolution of ¯hr through (30)

and (32). Thus, there exists an implicit dependence of bc on the second element of ξ2, i.e., Rhr.

For a better understanding of the modified isotropic
hardening law, we discuss a representative example of
magnetic cyclic loading with increasing amplitude in
Fig.4. Temporal variation of h/ms is shown in Fig. 4a
(inset). Specifically, we observe in Fig. 4a that ¯hr
in-creases from a
to b
. This increase in ¯hr results in the
evolution of the switching surface radius bcfrom a
to b
(see Fig.4b (inset)), which leads to the m– h response a
– b
in Fig.4b. Then, unloading from b
to d
(beyond
|h b
| = |h c
|) results in two distinct regimes. Firstly,
from b
to c
, h/ms remains less than the maximum
loading amplitude of the previous half cycle a
– b
, i.e.,
|h| < |h b
| = |h c
|. Thus, ¯hr _{remains constant between}

b

– c
, which results in bc to remain the same from b
to c
(see Fig.4b (inset)). In turn, going from c
to d
,
|h| > |h b
| = |h c
| of the previous half cycle a
– b
and
hence, ¯hr _{increases resulting to further increase of the}
switching surface radius in this regime (see Fig. 4b
(in-set)). The switching surface radius continues to increase
in a similar fashion during the subsequent half cycles.
e.g., d
– f
until eventually reaching bmax

c .

IV. THE EXTENDED CONSTITUTIVE MODEL FOR

ASYMMETRIC CYCLIC LOADING

So far in the proposed model, we incorporated the ef-fect of isotropic hardening during the initial magneti-zation. However, experiments show existence of minor

hysteresis loops under complex cyclic loading scenarios occuring after the initial magnetization. Clearly, from (29) and (32), we note that bc evolves either during the initial magnetization or when h−field increases beyond the previously maximum absolute value of |h| attained at a preceding cycle (see e.g. Fig.4). Nevertheless, fol-lowing available experimental observations, the switch-ing surface can shrink backwards if more complex mi-nor loop loadings are considered. In view of this, we at-tempt to enrich further the evolution law for bc to model more complex cyclic loading cases, especially when load-reversals may take place before the local |h| reaches the maximum h−field values attained in the preceding cycles.

A. Notion of a bounding surface

The approach followed to model such complex
mi-nor loops is closely related to the bounding surface idea
in mechanical plasticity. In particular, it has been
ob-served by Dafalias and Popov43 (see also Chaboche47)
in the context of mechanical plasticity that kinematic
and isotropic hardening is not enough to model cyclic
plasticity under complex loading conditions. In that
re-gard, Dafalias and Popov44 _{proposed a model where the}

evolution of the plastic internal variables (the remanent
internal variable hrin our case) depends additionally on
some discrete, history-dependent parameters associated
with loading/unloading of the material. These history
parameters are obtained in the present work by
con-structing a bounding surface in the hr _{space.} _{In the}
following, we first develop the notion of the bounds in
hrfor uniaxial loading/unloading and define the
history-dependent parameters. Subsequently, the notion is

ex-FIG. 4: (a) (inset) Cyclic loading profile. (a) Variation of ¯hr_{with time. (b) (inset) Evolution of b}

c with ¯hr. (b) Resulting hysteresis loop.

tended in the context of general three-dimensional mul-tiaxial loading/unloading cases.

A typical schematic representation of a hr–h loop,
ob-served in a uniaxial (1D) experiment is shown in Fig.5.
In this figure, the hr_{–h loop is observed to remain }
con-fined between two bounds: |hr_{| ≤ h}r

s, namely, an
up-per and a lower bound. It is observed that from an
initial energetic regime (| ˙hr| = 0), the remanent h-field
switches and eventually saturates to the corresponding
bound (|hr_{| = h}r

s), i.e, the lower bound for the loading
cycle and the upper bound for the unloading
half-cycle, as shown in Fig. 5 for an 1D loading example.
Studying numerous uniaxial experiments and following
Dafalias and Popov44 _{and Chaboche}47_{we conclude that}

the minor hysteresis loops can be modeled by
consider-ing bc to be a function of the proximity of the current
state of remanent field hr_{to the corresponding bounding}
(upper/lower) limit. This distance δ = AA0, as shown in
Fig.5is computed by

δ = hr_{s}+ sign( ˙h)hr. (33)

The proximity of a state of hr to the corresponding
bounding limit at the beginning of the pth _{half-cycle is}
denoted by δ(p). The illustrative example of Fig.5 shows
δ(p) for three half-cycles, namely p = 1, 2 and 3, which
together constitute a partially-reversed loading cycle.
These initial proximity parameters, δ(p), are the
history-dependent terms, which play a pivotal role in modeling
the evolution of bc for complex loadings. It is worth
not-ing that the initial local magnetization at the beginnnot-ing
of a new half-cycle also plays a crucial role in the
mi-cromagnetic model of Fulmek and Hauser61, which also
models the minor loops by evolving a history-dependent
material parameter. The same notion of evolving the

FIG. 5: Schematic illustration of upper and lower bounds, δ and δ(p) for the uni-axial loading case.

history-dependent coercive field bc is considered in our model, but within the framework of the bounding sur-face idea, which is by default a three-dimensional frame-work and in principle can also be extended to anisotropic magnetic responses.

In this regard, the computation of δ for the multiaxial
case is a bit more involved but otherwise a direct
exten-sion of the above described 1D case. For simplicity, we
assume an isotropic magnetic response to obtain a
spher-ical bounding surface B in the hr space of diameter 2hr_{s}
(see Fig. 6a). To obtain δ, we first construct a plane

FIG. 6: (a) Schematic illustration of the bounding surface B and the circle C on the plane containing the vectors n_{h}˙
and hr_{. (b) Estimation of δ}

(p) from the planar geometry on C.

containing both the vectors hr_{and n}
˙

h= ˙h/| ˙h| and com-pute θ = cos−1(hr· nh˙/|h

r_{|). The intersection of this}
plane with B leads to a circle C, whose 3D view and the
2D projection are shown in Fig. 6a and b, respectively.
Now, δ is obtained by computing the Eucledian distance
between AA0, where A represents the current state of
hr and A0 is the corresponding point on B obtained by
extending a straight line from A in the direction of n_{h}˙
(see Fig.6b). From the planar geometry on the circle C
(Fig.6b) with center O and radius hr

s, we obtain δ using straightforward geometrical arguments as

δ = q

(hr

s)2− |hr|2sin

2_{θ + |h}r_{| cos θ.} _{(34)}
Figure6b shows that the uniaxial loading and unloading
cases presented in Fig.5and defined via the equation (33)
are special cases of the more general three-dimensional
framework that can be obtained by setting θ = 0 and π,
respectively, in equation (34).

By summarizing the above discussion, one may define the history-dependent variables to form a set of size 2p + 4, i.e.,

ξ2p+4≡ {¯hr, Rhr, ¯he, δ, δ_{(p)}, ¯he_{(p)}, δ_{(p−1)}, ¯he_{(p−1)}, ..., δ_{(1)}, ¯he_{(1)}},

where p is the number of half cycles (including the current
one), and ¯he_{is the accumulated energetic h-field (defined}
later in (38), similar to ¯hr_{). Finally, ¯}_{h}e

(p) is the ¯h
e_{at the}
beginning of the pth_{half-cycle (similar to δ}

(p)). In
princi-ple, ξ is a set that has a continuously increasing number
of elements, starting from ξ6≡ {¯hr, Rhr, ¯he, δ, δ_{(1)}, ¯he_{(1)}}.

Fortunately, real materials exhibit a fading memory43,44_{.}

As a result, one can consider gradually increasing relative weights on δ(p), δ(p−1), δ(p−2) and so on and eventually discard the oldest history variables. A specific functional

form of bc(ξ2p+4) is proposed next based on available ex-perimental observations.

It should be noted that in the general context of mag-netically anisotropic materials the bounding surface B is expected to become non-spherical albeit remain convex. The proposed framework can be readily extended for such cases but would probably require additional variables and anisotropic invariants.

B. First order minor loops

Typical experiments39,40,62 _{show that the first order}

minor loops (FOMLs) exhibit, in a sense, two distinct
features; (i) a low |h| switching depends on the
load-ing/unloading history while (ii) the switching surface
ra-dius increases from bc to bmaxc during subsequent
switch-ing. When a load reversal takes place at a |h| < hs,
both the rotation of the magnetic domains in the
pre-vious loading direction and the pinning of domain walls
remain incomplete. Thus, one observes switching at a
lower |h| during the current half cycle because of partial
rotation of the magnetic domain walls during the
pre-vious half cycle57_{. Then, as switching proceeds during}

the current half cycle, the domain walls get rotated and pinned in the direction of |h|, as usual. This micromag-netic phenomenon is captured in the present phenomeno-logical model as follows; bc is allowed to decrease during the energetic response of a partially-reversed half-cycle, whereby it may increase up to bmax

c during a subsequent switching. By recalling the observations (i) and (ii) done previously, we combine all the previous constitutive equa-tions for bc and extend them into three distinct evolu-tion laws for the switching surface for the three different

regimes – (i) the initial magnetization, (ii) the energetic part, and (iii) the switching part of a half cycle. Each one of these regimes is considered independently in the present work and their modeling can be carried sepa-rately depending on the level of complexity one is willing to reach.

Specifically, the initial magnetization regime is indi-cated by a function

K = H( ˙¯hr), (35) which is essentially a Heaviside step function with K = 1 during the initial magnetization and 0 otherwise.

Simi-larly, the energetic and the switching regimes of a half-cycle are written in terms of a Heaviside step function as J = 1 − H 1 − δ δ(p) , (36)

Recall from Section IV A that δ = δ(p) during the en-ergetic response and δ starts decreasing from δ(p) when the switching starts. Thus, from definition (36), we have J = 1 and 0 to represent the energetic and the switching regimes, respectively. We now propose a combined evo-lution law for bc depending on the indicator functions K and J such that

bc=
bmaxc
tanh
_{¯}
hr
¯
hr
0
81/q
if K = 1
b(0)c
1 − k1
1 −δ(p)
2hr
s
Rhr
hr
s
F1
if K = 0, J = 1
b(0)c +
bmax
c
tanh
¯_{h}r
¯
hr
0
81/q
− b(0)c
F2 if K = 0, J = 0,
(37)

where k1 is a material parameter, b (0)

c is the initial bc at the beginning of the energetic/switching regime, while the first law corresponding to the initial magnetization is the one proposed in (29).

The functionsF1andF2are used to ensure a smooth
decrease/increase in bc during the energetic and
switch-ing parts, respectively, of a partially-reversed half-cycle.
Note that during the energetic response, i.e., when the
switching surface is modeled to shrink following (37)_{2},
both the accumulated remanent field ¯hrand the
proxim-ity parameter δ remain constant. Thus, the evolution of
F1 during the energetic response may be carried out in
terms of an accumulated energetic h-field, defined as

˙¯he_{=}p ˙he_{· ˙h}e_{,} ¯_{h}e_{=}
Z

t

˙¯he_{dt.} _{(38)}
A straightforward choice is to consider F1 to be a
satu-ration function, which evolves from 0 and saturate at 1,
such as
F1= tanh
_{δ}D
(p)
2Rhr
_{h}¯e
¯
he
0
−
¯
he
(p)
¯
he
0
, (39)

where the term ¯he

(p) is a history-dependent parameter,
that is ¯he at the beginning of the pth half cycle (similar
to δ(p)) and δ(p)D = δ(p)+ δ(p−1)− 2hrsis the proximity of
the pth _{half-cycle to the (p − 1)}th _{one, i.e., the proximity}
between two subsequent half-cycles. Finally, ¯he0in (39) is
a material parameter that represents a reference
accumu-lated energetic h-field (similar to ¯hr

0 in (29)). Similarly,

F2 is chosen to be a saturation function, that evolves from 0 to 1, such that

F2= tanh
(
k2
2hr
s
δM
1 − δ
δ(p)
_{δ}D
(p)
2hr
s
−k3)
, (40)

where k2and k3are positive parameters that dictate the shape of the minor loop, and

δM = max{δ(1), δ(2), ..., δ(p)}.

Note that F2 may become singular in the degenerate case of δD

(p) → 0, i,e. for tiny minor loops due to small
fluctuations in the local h. This can remedied by adding
a correction term in (37)_{2}. Such a correction is shown in
AppendixVIIIbut is not necessary for well-defined cyclic
loads. The use of (37) to modeling the FOMLs – arising
due to partially-reversed loading cycles is discussed next
by use of two typical examples.

A typical example of a first-order reversal curve is
de-picted in Fig.7. The inset of Fig.7a shows the
uniax-ial loading profile, where a
– b
represents the initial
magnetization of a virgin sample followed by a
partially-reversed cycle b
– d
– f
. The initial magnetization
from a
to b
results in the corresponding evolution of bc
as evaluated from (37)_{1}(see Fig.7a). The corresponding
response in the m – h space is shownfor the same regime
in Fig.7b.

At the beginning of the second half-cycle b
– d
, we
have δ(2) ≈ 2hrs and b
(0)
c = bmaxc {tanh[(¯h
r_{/¯}_{h}r
0)
8_{]}}1/q_{.}
Thus, the evolution law for bc, i.e, (37)_{2} reduces to

FIG. 7: (a) (inset) Cyclic loading profile. (a) Evolution of bc in time. (b) Resulting m – h loop.

bc = b (0)

c , resulting in a constant bc between b
– c
.
During subsequent switching, bc evolves following (37)_{3}.
Note in (37)_{3} that the coefficient ofF2 now vanishes as
bc did not decrease from bmaxc . Hence, (37)2 and (37)3
together ensure a constant bcon unloading if the
preced-ing loadpreced-ing goes beyond saturation (see Fig. 7a).
Con-sequently in Fig.7b, we obtain a m – h response in the
interval b
– c
coinciding with the major loop.

The path d – f represents a partially-reversed half-cycle, where the load reversal takes place before satu-ration at d and thus, δ(3) < 2hrs. During the ener-getic response, d – e , bcdecreases to values lower than b(0)c = bmaxc following the constitutive expression (37)2 (see Fig.7a). Consequently, the switching is initiated at

e

at values lower than bmax

c . From that point on, bc
starts evolving following (37)_{3} and hence increases from

e

to f approaching bmax

c . The resulting m – h response is shown by the segment d – e in Fig.7b.

Note that the shape of the minor loop d – e depends explicitly on the choice of the minor loop shape param-eters k1, k2 and k3. The identification of k1, k2 and k3 by use of a least-square fitting of the model with avail-able experimental data is discussed in SectionV. On the other hand, the proposed forms of the functionsF1 and F2will be shown to be sufficient to model a large number of different magnets.

For completeness, we also investigate a more compli-cated loading scenario where initially the magnet is not magnetized to saturation. That is a very important case in particle-filled magnetorheological elastomers, whereby not all particles attain the same level of magnetization given an external overall magnetic applied field.

In particular, the loading profile is depicted in the inset of Fig.8a. In this case, an initial loading from a to b increases bc up to a given value bc(1) resulting to an

ini-tial magnetization response in the same shown in Fig.8b.
The subsequent two half cycles b
– d
and d
– f
fol-low the evolution equations (37)_{2} and (37)_{3} during the
corresponding energetic and switching regimes,
respec-tively, and result in a m – h response, shown in Fig.8b.
An interesting observation can be made during the last
unloading half-cycle f
– i
. We notice from Fig.8a
(in-set) that |h| exceeds hmax when the magnet is unloaded
beyond h
. Thus, the shrinkage f
– g
of the switching
surface is followed by its expansion in two steps. First,
we get the expansion from g
to h
evaluated by
equa-tion (37)_{3}. This is followed by an expansion of bc in the
interval h
to i
as computed by equation (37)_{1}. As a
result, we observe a two step magnetization response g
– i
in Fig.8b. Therefore, three different regimes are
ob-tained from relation (37) during a half-cycle for a loading
condition in the interval f
– i
.

Accurate prediction of the higher-order minor loops
necessitates a more tedious definition of bc and, in
gen-eral, it requires a metric to identify the order of the minor
loop. On the other hand, the nature of evolution of bc
re-mains the same for the higher order loops except for the
need of additional history-dependent terms. Thus, an
efficient storage of the order of the minor loop and the
set ξ requires a suitable computational algorithm, which
is beyond the scope of this paper. However, typically
in engineering applications with magnets63_{and MREs}64_{,}

the material is not loaded with a highly fluctuating mag-netic field that may cause secondary or higher order mi-nor loops. Thus, the proposed model that captures ac-curately the FOMLs, is expected to be sufficient for the applications at hand.

FIG. 8: (a) (inset) Cyclic loading profile. (a) Evolution of bc in time. (b) Resulting m – h loop.

V. ASSESSMENT OF THE MODEL WITH

EXPERIMENTS

In this section, we use the proposed model to probe
and predict a large number of experimental data
avail-able in the literature. The number of model parameters
to be specified depends on the complexity of the
exper-iment we intend to model. For the most general case
which involves modeling a magnet accurately up to its
first-order minor loops, we need to specify eleven
param-eters, namely, χ(r)_{, K}

1, hrs, κ, bmaxc , ¯h0r, ¯he0, q, k1, k2 and
k3. On the other hand, modeling only the major loop
requires five material parameters, namely χ(r)_{, K}

1, hrs, κ, and bmaxc with all others to remaining inconsequential. Modeling the initial magnetization response along with the major loop requires two additional parameters ¯hr

0and q. Finally, for the modeling of the minor loops, we need to specify the remaining ¯he

0, k1, k2 and k3constants. In this regard, we carry out a least square fitting of the model parameter to available experimental data in three steps.

i We first find the optimal major loop parameters ¯bmax_{c} ,
χ(r)_{, ¯}_{K}

1 and hrs by using the lsqcurvefit function
in MATLAB65_{. For simplicity, we manually select}

κ = 0 or 1, depending on the nature of the hysteresis loop.

ii We, then, find the initial magnetization parameters q and ¯hr0 using the same function.

iii Finally, we identify the rest of the four minor loop
parameters, namely, ¯he_{0}, k1, k2 and k3 if such
infor-mation are available from the experiments analyzed.
It is useful at this point to write down the simple form
of our model in the case of uniaxial loading (say, along

e1) of isotropic magnets, which corresponds to most ex-periments in the literature and those analyzed in the fol-lowing. Thus, (6) becomes

b = µ0

(1 − χ(r)_{)}(h − h
r

), (41)

The magnetization is then computed from

µ0m = b − µ0h = µ0
_{1}
(1 − χ(r)_{)}(h − h
r_{) − h}
, (42)

while the uniaxial remanent field is obtained from

br= µ0
(1 − χ(r)_{)}
h + ¯K1f
hr
hr
s
. (43)

Here, ¯K1= K1(1−χ(r))/µ0and f (hr) are defined in (24). Consequently, the switching surface (19) now becomes

φ := (br)2− µ
2
0
(1 − χ(r)_{)}2
¯
b2_{c}. (44)

We compute hr _{from an associated switching rule, }
ob-tained from the above using the classical radial return
algorithm by Ortiz and Simo66. The algorithm used in
our computations is detailed for completeness in the
Ap-pendix.

In the following, we compare the proposed model with
the uniaxial tests of (a) sintered NdFeB magnets by
Huang et al.6 _{and (b) NdFeB powders by Deng et al.}5

and P´erigo et al.4. In those examples, we model the
initial magnetization and the major loop. Subsequently,
we compare the proposed model with the experimentally
observed minor loops by W lodarski39 _{and Liu et al.}3_{.}

It is important to mention that the polycrystalline mag-nets, used in the corresponding experiments, are typi-cally isotropic. Anisotropic magnets may be manufac-tured through dedicated manufacturing techniques and

will require additional constitutive parameters that will allow to describe properly the preferred magnetization directions.

A. Sintered NdFeB magnets

Sintered NdFeB magnets are the classical example of nucleation-type magnets with high initial susceptibility. In Fig. 9 we obtain two sets of experimental data from Huang et al.6 – (a) the major hysteresis loop for spark plasma sintered NdFeB magnets, where the solid magnet is obtained by sintering very fine melt-spun NdFeB rib-bons of less than 40 µm diameter, and (b) the major loop for sintered NdFeB, prepared by sintering coarse NdFeB ribbons (greater than 40 µm diameter).

We obtain a least-square fit of our model with the ex-perimental data in Fig. 9a in two steps. First, we fit the outer loop of the experiment and obtain the opti-mal ¯bmax

c , χ(r), ¯K1 and hrs as shown in Table 1. Next,
the model is fitted to the experimental initial
magneti-zation response to obtain ¯hr_{0} and q as shown in Table I.
The minor loop parameters ¯he

0 k1, k2 and k3 are incon-sequential and hence, are set to ¯he

0 = 1.0 MA/m and k1= k2= k3= 0 due to unavailability of any minor loop data.

TABLE I: Material parameters for sintered NdFeB mag-nets

χ(r)= 0.0748 K¯1= 0.28 MA/m

hr_{s}= 0.65 MA/m κ = 0.0

¯_{b}max

c = 1.20(a) | 1.52(b) MA/m ¯hr0= 0.58 MA/m

q = 3.35 ¯he

0= 1.0 MA/m

k1= 0.0 k2= 0.0

k3= 0.0

We observe that the present model is capable of probing
accurately the experimental data in Fig. 9a. Here, we
note that in addition to modeling the major loops, the
present model also traces accurately the initial
magne-tization response. Note that the simple switching
sur-face models of Landis14_{and Kinkel}15_{, shown for }

compar-ison as well as the pseudo-particle models only model the outer coercive loops accurately. Next, we probe the hys-teresis loop for a coarse-grained sintered NdFeB magnet in Fig. 9b. The model is able to reproduce this second case by only re-identifying the parameter bmax

c , keeping
the rest of the parameters the same. Thus, it is observed
that, different variants of magnets made of the same
ma-terial (e.g., exhibiting different grain sizes) can be
mod-eled by a small variation of the coercive field bmax_{c} .

B. NdFeB powder

In Fig.10, we consider the experimental data of Deng
et al.5 _{and P´}_{erigo et al.}4 _{for quasi-static, uniaxial }

load-ing of melt-spun NdFeB powder samples. In both cases, the proposed model is capable of reproducing extremely well the corresponding experimental data (see TableIIfor corresponding parameters). Specifically, we first identify the model parameters using the experimental results of Deng et al.5. Then, the experiments of P´erigo et al.4are probed by re-adjusting ¯K3 and χ(r), which serve to de-scribe the shape of the hysteresis loop. TableII displays the values of the model parameters, used to describe the major hysteresis loop. Note that in both experiments the maximum coersive field bmaxc is identical.

TABLE II: Material parameters for NdFeB powder

χ(r)= 0.095(a) | 0.163(b) K¯1= 0.078(a) | 0.15(b) MA/m
hr_{s}= 0.67 MA/m κ = 1.0
¯_{b}max
c = 0.766 MA/m ¯hr0= 0.551 MA/m
q = 17.5 ¯he
0= 1.0 MA/m
k1= 0.0 k2= 0.0
k3= 0.0

In addition, use of the same initial magnetization param-eters ¯hr

0 and q allows us to recover accurately the initial magnetization response in both samples. In Fig.10, the parameter q implies that the coercivity in NdFeB powder samples can be attributed to a combined effect of nucle-ation and pinning, which is in agreement with recent mi-croscopic observations by Liu et al.67 in NdFeB ribbons (from which the NdFeB powders are obtained through grinding). Finally, the four minor loop parameters ¯he

0, k1, k2 and k3are inconsequential due to unavailability of any minor loop data and thus are set to ¯he

0= 1.0 MA/m and k1= k2= k3= 0.

C. MgMn steel

In Fig11, we use the complete model to probe the
ex-perimental data of W lodarski39 _{for MgMn steel, which}

include several fully-reversed, uniaxial hysteresis loops with different amplitudes of loading. Thus, in addition to the initial magnetization and major coercive loop, the latter experiments provide also information on symmet-ric minor loops. We first identify ¯bmax

c , χ(r), ¯K1 and hrs in order to probe the experimental major loop (see Ta-bleIII).

TABLE III: Material parameters for MgMn Steel

χ(r)= 0.9913 K¯1= 9.5 A/m
hr
s= 1583.0 A/m κ = 0.0
¯_{b}max
c = 72.0 A/m ¯hr0= 1451.0 A/m
q = 45.6 ¯he
0= 98.7 A/m
k1= 3.0 k2= 2.5
k3= 0.1

Subsequently, we fit the initial magnetization response by identifying the parameters q and ¯hr

FIG. 9: Experimental m-h response of a NdFeB magnet6 _{with the fitted rate-independent proposed model.}

FIG. 10: Experimental m-h response of NdFeB powder from (a) Deng et al.5 and (b) P´erigo et al.4 with the fitted rate-independent proposed model.

the model with one of the minor loop data to obtain ¯

he

0, k1, k2 and k3 as shown in TableIII. In Fig. 11b, we use the already identified model to predict two additional experimental minor loops. We thus show that the model is able to reproduce but also predict sufficiently well the major and minor hysteresis loops of MgMn steel.

D. Asymmetric minor loops

In Fig. 12, we use our model to probe the experimen-tal data for two different magnets; (a) annealed

nanocrys-talline Co alloy and (b) 3% silicon steel, subjected to
uni-axial, partially-reversed loading, which results in
asym-metric minor loops. The experimental m – h response
along with three first-order reversal curves (FORCs) for
the annealed nanocrystalline Co alloy magnet is obtained
by Mart´ınez-Garc´ıa et al.62. Similar to the previous
fig-ures, we carry out a two step fitting of our model. First,
we fit the major loop data of Mart´ınez-Garc´ıa et al.62 _{to}

obtain the model parameters except ¯hr

0 and q, which are inconsequential due to unavailability of the initial mag-netization data. We then use the model to probe one of the experimental FORC data thus identifying the

pa-FIG. 11: Experimental m-h response of MgMn Steel by W lodarski39 _{with (a) the fitted model and (b) the model}

predictions.

rameters ¯he

0, k1, k2 and k3. The resulting values for the model parameters are given in TableIV.

TABLE IV: Material parameters for annealed
nanocrys-talline Co alloy
χ(r)_{= 0.855} _{K}_{¯}
1= 0.718 kA/m
hrs= 51.5 kA/m κ = 1.0
¯_{b}max
c = 9.978 kA/m ¯hr0= 1.0 A/m
q = 100.0 ¯he_{0}= 85.0 A/m
k1= 4.0 k2= 1.85
k3= 1.25

In Fig. 12a, the solid lines correspond to the model re-sponse that is fitted to the corresponding experimental data. The dashed lines correspond to predictions of the model without introduction of additional model param-eters.

Finally, Fig.12b shows the experimental data of
Ben-abou et al.40_{corresponding to the b – h response of a 3%}

silicon steel sample, that is subjected to a periodic h-field
with the superposition of third harmonics. This type of
loading gives rise to asymmetric minor loops. Again, a
two-step fitting procedure, consisting of fitting the major
loop and only one of the minor loops from the
experi-mental data, yields the corresponding model parameters
(see TableV). Note again that the initial magnetization
parameters ¯hr_{0} and q remain inconsequential due to
un-availability of the initial magnetization data and thus are
set equal to 1 and 0, respectively. The second minor loop
is then found to be well predicted by the proposed model.

TABLE V: Material parameters for 3% silicon steel

χ(r)_{= 0.999} _{K}¯_{3}_{= 12.5 A/m}
hr
s= 1000 A/m κ = 1.0
¯_{b}max
c = 41.0 A/m ¯hr0= 1.0 A/m
q = 100.0 ¯he
0= 100.0 A/m
k1= 8.0 k2= 4.0
k3= 1.34

The examples presented in this section illustrate the capabilities of the model to reproduce and predict mag-netic responses obtained by very complex loading histo-ries and specifically resulting to asymmetric minor loops.

VI. FORC DIAGRAMS

VII. CONCLUDING REMARKS

In the present study, we propose a rate-(in)dependent constitutive model for magnetic hysteresis in terms of a nonlinear convex Helmholtz free energy and a convex dis-sipation potential. Qualitative connections with existing micromagnetic domain theories are discussed throughout the study. In the limit of rate independent response, the dissipation potential leads to the switching surface (sim-ilar to the yield surface in mechanical plasticity). We incorporate the effect of initial magnetic hardening of a virgin specimen by introducing an isotropic hardening law, leading to the gradual growth of the switching sur-face until reaching a limiting sursur-face, which encapsulates all the internal switching surfaces during the magnetiza-tion/demagnetization. Symmetric and asymmetric mi-nor loops are modeled by introducing a set of discrete, history-dependent thermodynamic variables, that control the shrinkage and expansion of the switching surface

de-FIG. 12: (a)(inset) Loading profile for FORCs. (a) Experimental m-h response for nanocrystalline Co alloy from Mart´ınez-Garc´ıa et al.62 with the model fitting and predictions. (b)(inset) Loading profile and (b) experimental b-h

response for 0.3% silicon steel by Benabou et al.40 with the fitted model. Time scale is irrelevant for the rate-independent model.

pending on the loading history and the state of
magneti-zation. In this context, we utilize the existing framework
of the bounding surface (originally used in the context
of mechanical plasticity) and extend it to describe the
macroscopic response of permanent magnets. In
particu-lar, the present natural extension of the existing
switch-ing surface framework of McMeekswitch-ing and Landis13_{, }

Lan-dis14 _{and Klinkel}15 _{enables us to model accurately the}

initial magnetization and the symmetric and asymmetric minor loops up to first order.

One of the key advantage of the present model is the sequential increase in the model complexity depending on the experiment we intend to model. Modeling only the major hysteresis loop does not require any isotropic hardening or shrinkage/expansion of the switching sur-face depending on the loading history. Hence, only the four material parameters related to the coercive field and the shape of the major loop are sufficient to describe the major hysteresis loop. On the other hand, if one needs to model also the initial magnetization response, two ad-ditional hardening parameters are further considered.

The modeling of the minor hysteresis loops necessi-tates a more tedious definition of the switching surface depending on the state of magnetization and the loading history, whereas it requires the determination of three additional material parameters. This sequential increase in the model complexity also allows us to probe various experimental data by identifying the model parameters in multiple independent steps. In the present work, we use at most eleven model parameters to probe the most com-plex experimental loading history corresponding to first order asymmetric minor loops (FOMLs). This makes the corresponding parameter identification a well-controlled

and fairly straightforward task contrary to the pseudo
particle model31,42_{, which requires 30 to 50 parameters}

that need to be identified all at once.

Specifically, the model has been used to probe and predict several experimental data including the m–h re-sponses of the purely nucleation-type sintered NdFeB magnets, the combined nucleation-pinning-type NdFeB powder samples, the annealed nanocrystalline Co alloy and the b–h responses of the MnMg steel and the 3% Si steel. Symmetric and asymmetric minor loop data from different experiments are used to probe the effectiveness of the proposed evolution/shrinkage law for the coercive field bc. Excellent recovery and whenever available also excellent prediction of available experiments is obtained in the present study.

The model can be extended further to model the
rate-dependent response of hard magnets by considering the
dissipation potential to be the same power law with
0 < n ∞ along with some additional terms
incorporat-ing the eddy current and the anomalous loss. Anisotropic
polycrystal or single crystal magnets with a preferred
di-rection can be modeled by a straightforward extension of
the present framework, by following ideas analogous to
the Hill and single-crystal mechanical plasticity. In
addi-tion, the present model is a first step towards analyzing
the response of magnetorheological elastomers made of
permanently magnetized particles subjected to complex
magnetic and mechanical loading histories (see the very
recent work of Kalina et al.42 _{in this direction). Finally,}

the proposed framework is fairly general and uses vec-torial quantities thus allowing its full three dimensional implementation in numerical schemes (such as the finite elements or fast Fourier transform methods).

VIII. ACKNOWLEDGEMENTS

This work was supported by the European Research Council (ERC) under the European Unions Horizon 2020 research and innovation program (grant agreement No 636903 - MAGNETO).

APPENDIX A

In this section, we describe the numerical integration of
the proposed model. We assume that the state of
magne-tization is fully known at the time tn. For an increment in
the h-field ∆h, the state of the magnet at tn+1= tn+ ∆t
is sought to be determined. We employ the radial return
algorithm by Ortiz and Simo66 to obtain the increment
in the remanent field ∆hr_{corresponding to ∆h.}

The determination of ∆hr _{requires defining an }
asso-ciated magnetic switching rule, which we obtain by first
defining the total Lagrangian:

L = −br_{· ˙h}r_{+ ˙λφ(b}r_{, ¯}_{h}r_{, ξ}

N), (A.1)

where ˙λ is the Lagrange multiplier. Now, the minimiza-tion of L leads to the Kuhn-Tucker condiminimiza-tions

˙

hr= ˙λ ∂φ

∂br = 2 ˙λb

r_{,} _{(A.2)}

with ˙λ = 0 for φ < 0 and ˙λ > 0 for φ = 0, where the above represents the associated switching rule, which is equivalent to the associated flow rule in mechanical plasticity. Thus, the evolution of hr is computed from (A.2) while ˙λ > 0 together with the application of the constraint φ = 0.

We use an unconditionally stable backward Euler
iter-ation method to solve (A.2) in time15,16_{. We note that}

during the energetic response, i.e., when φ(br_{, b}
c) < 0,
the condition ˙λ = 0 reduce (A.2) to ˙hr = 0. Hence, hr
at tn+1is simply

hr_{n+1}= hr_{n}. (A.3)

Thus, we see that hr_{remains constant at the time of the}
energetic response. During the magnetic switching, i.e.
φ(br_{, b}

c) = 0, (A.2) is expressed as

hr_{n+1}= hr_{n}+ 2γnbrn, (A.4)

where γn= ˙λ(tn− tn−1), and the residues, corresponding to (A.2) and (19) are calculated as

ra= hrn+1− h r n− 2γnbrn (A.5) and rb= brn+1· b r n+1− {bc(ξ2p+4(n))}2, (A.6) respectively. The above two equations together forms a 4×1 residue vector R = [ra, rb]T. Note that, in (A.6) the

switching surface radius bcis a function of 2p + 4 history-dependent parameters, which are stored up to the nth increment. Thus, the bc in the n + 1th increment is ob-tained from the history variables, stored at the previous increment.

Now, if the residue norm ||R|| is greater than a pre-scribed tolerance value, we need to correct gn+1 = [hr

n+1, γn+1]T from a local Newton iteration, which can
be accomplished by calculating ∆g = [∆hr_{, ∆γ]}T _{from}
the following

G(k)_{n+1}∆g = −R(k), (A.7)

where G(k)_{n+1}= ∂R(k)/∂gn+1is a 4 × 4 matrix. Next, the
gn+1is modified after kth local Newton iteration as

g(k+1)_{n+1} = g_{n+1}(k) + ∆g. (A.8)

This local iteration continues until ||R||(k+1) becomes less than the prescribed tolerance.

APPENDIX B

It is observed that a singularity may appear in equation
(37)_{3} in the degenerate case of δD

(p) → 0. To overcome
this problem, one may augment (37)_{2} with an additional
term, such as
bc(p)= b(0)c
1 − k1
1 − δ(p)
2hr
s
Rhr
hr
s
F3F1
+
bmaxc
tanh
_{¯}
hr
¯
hr
0
1/q
− bc(0)
(1 −F3)F4,
(B.1)

where the functionsF3 andF4 are now defined by
F3= tanh
6.0δ
D
(p)
hr
s
, (B.2)
F4= tanh
(
2Rhr
δD
(p)
_{¯}_{h}e
¯
he
0
−
¯
he
(p)
¯
he
0
)
, (B.3)

respectively. Now, for δD

(p) = 0, F3 vanishes, reducing (B.1) to its second term only. Therefore, instead of de-creasing, the bcrather increases to bmaxc during the ener-getic response by virtue of the saturation functionF4.

1_{G. C. Hadjipanayis and W. Gong,} _{Journal of Applied Physics}

64, 5559 (1988).

2_{Z. Gao, D. C. Jiles, D. J. Branagan,} _{and R. W. McCallum,}

Journal of Applied Physics 79, 5510 (1996).

3_{Z. Liu, H. Huang, X. Gao, H. Yu, X. Zhong, J. Zhu, and D. Zeng,}

Journal of Physics D: Applied Physics 44, 025003 (2010).

4_{E. P´}_{erigo, M. de Campos, R. Faria, and F. Landgraf,}_{Powder}

technology 224, 291 (2012).

5_{X. Deng, Z. Liu, H. Yu, Z. Xiao,} _{and G. Zhang,} _{Journal of}